|Name, symbol||indium, In|
|Appearance||silvery lustrous gray|
|Indium in the periodic table|
|Atomic number (Z)||49|
|Group, block||group 13, p-block|
|Element category||post-transition metal|
|Standard atomic weight (±) (Ar)||114.818(1)|
|Electron configuration||[Kr] 4d10 5s2 5p1|
|2, 8, 18, 18, 3|
|Melting point||429.7485 K (156.5985 °C, 313.8773 °F)|
|Boiling point||2345 K (2072 °C, 3762 °F)|
|Density near r.t.||7.31 g/cm3|
|when liquid, at m.p.||7.02 g/cm3|
|Triple point||429.7445 K, ~1 kPa|
|Heat of fusion||3.281 kJ/mol|
|Heat of vaporization||231.8 kJ/mol|
|Molar heat capacity||26.74 J/(mol·K)|
|Oxidation states||3, 2, 1, −1, −2, −5 (an amphoteric oxide)|
|Electronegativity||Pauling scale: 1.78|
|Ionization energies||1st: 558.3 kJ/mol
2nd: 1820.7 kJ/mol
3rd: 2704 kJ/mol
|Atomic radius||empirical: 167 pm|
|Covalent radius||142±5 pm|
|Van der Waals radius||193 pm|
|Speed of sound thin rod||1215 m/s (at 20 °C)|
|Thermal expansion||32.1 µm/(m·K) (at 25 °C)|
|Thermal conductivity||81.8 W/(m·K)|
|Electrical resistivity||83.7 nΩ·m (at 20 °C)|
|Young's modulus||11 GPa|
|Brinell hardness||8.8–10.0 MPa|
|Discovery||Ferdinand Reich and Hieronymous Theodor Richter (1863)|
|First isolation||Hieronymous Theodor Richter (1867)|
|Most stable isotopes of indium|
|Decay modes in parentheses are predicted, but have not yet been observed|
Indium is a chemical element with symbol In and atomic number 49. It is a post-transition metallic element that is rare in Earth's crust. The metal is very soft, malleable and easily fusible, with a melting point higher than sodium, but lower than lithium or tin. Chemically, indium is similar to gallium and thallium, and it is largely intermediate between the two in terms of its properties. It has no obvious role in biological processes and common compounds are not toxic. It is most notably used in low melting point metal alloys such as solders, soft metal high vacuum seals, and in the production of transparent conductive coatings of indium tin oxide (ITO) on glass.
- 1 Properties
- 2 Chemical compounds
- 3 Biological and medical functions
- 4 Creation
- 5 History
- 6 Production
- 7 Applications
- 8 Health issues
- 9 See also
- 10 References
- 11 External links
Indium is a very soft, silvery-white, highly ductile, relatively rare post-transition metal with a bright luster. It is so soft (Mohs hardness 1.2) that the metal can be cut with a knife, as can sodium. It also leaves a visible line on paper. Like tin, when it is bent indium emits a high-pitched "cry". Like gallium, indium is able to wet glass. Like both, indium has a low melting point, 156.60 °C (313.88 °F); higher than its lighter homologue, gallium, but lower than its heavier homologue, thallium, and lower than tin. Only mercury, gallium, and most of the alkali metals have lower melting points. Its boiling point is 2072 °C (3762 °F), higher than that of thallium, but lower than that of gallium, showing opposition to the melting points' trend. Indium thus has a very large liquid range of around 2000 °C. The density of indium, 7.31 g·cm−3, is also higher than that of gallium, but lower than that of thallium. Below its critical temperature of 3.41 K, indium becomes a superconductor. At standard temperature and pressure, indium crystallizes in the tetragonal crystal system in the space group I4/mmm (lattice parameters: a = 325 pm, c = 495 pm).
Indium metal does not react with water, but it is oxidized by stronger oxidizing agents, such as halogens to give indium(III) compounds. It does not form a boride, silicide or carbide, and the hydride InH3 has only a transitory existence, even at low temperatures, before reverting to the elements.
Indium has 39 known isotopes, ranging in mass from 97 to 135. Only two isotopes occur naturally in primordial nuclides: indium-113, the only stable isotope, and indium-115, which has a half-life of 4.41×1014 years, four orders of magnitude longer than the age of the universe and nearly 50,000 times longer than that of natural thorium. Indium-115 makes up 95.7% of all indium.
The most stable artificial indium isotope is indium-111, which has half-life of approximately 2.8 days. All other isotopes have half-lives shorter than 5 hours. Indium also has 47 meta states; indium-114m1 is the most stable, being more stable than the ground state of any indium isotope other than the primordial ones.
Indium has 49 electrons, having an electronic configuration of [Kr]4d105s25p1. In its compounds, indium most commonly loses its three outermost electrons, becoming indium(III) ions, In3+, but in some cases the pair of 5s-electrons do not ionize, resulting in indium(I), In+. The stabilization of the monovalent state is attributed to the inert pair effect, the stabilization of 5s-orbital due to relativistic effects, which are greater for heavier elements. Thallium (indium's heavier homolog) shows an even stronger effect, making oxidation to thallium(I) more likely than to thallium(III), making +1 the more likely oxidation state, whereas gallium (indium's lighter homolog) commonly shows only the +3 oxidation state. Thus, although thallium(III) is a moderately strong oxidizing agent, indium(III) is not, and indium(I) compounds are often powerful reducing agents.
A number of standard electrode potentials, depending on the reaction under study, are reported for indium:
|−0.40||In2+ + e−||↔ In+|
|−0.49||In3+ + e−||↔ In2+|
|−0.443||In3+ + 2 e−||↔ In+|
|−0.3382||In3+ + 3 e−||↔ In|
|−0.14||In+ + e−||↔ In|
Indium(III) oxide forms when the element is burned in air or when the hydroxide or nitrate is heated. In2O3 adopts a structure like alumina. It is amphoteric, i.e., it can react with both acids and bases. Its reaction with water results in insoluble indium(III) hydroxide, which is also amphoteric, reacting with alkalis to give indates(III) and with acids to give indium(III) salts:
- In(OH)3 + 3 HCl → InCl3 + 3 H2O
Indium forms the expected trihalides. Chlorination, bromination, and iodination of In gives, respectively, colorless InCl3 and InBr3, and yellow InI3. The compounds are Lewis acids, somewhat akin to the better known aluminium trihalides. Again like the related aluminium compound, InF3 is polymeric.
See also Indium halides
Indium(I) compounds are not common. The chloride, bromide, and iodide are deeply colored, unlike the parent trihalides from which they are prepared. Other In(I) compounds include a sulfide. Indium(I) sulfide is the product of reaction between indium and sulfur or indium and hydrogen sulfide, and can be received at 700—1000 °C. Indium(I) oxide black powder is received at 850 °C during reaction between indium and carbon dioxide or during decomposition of indium(III) oxide at 1200 °C. Cyclopentadienylindium(I), which was the first organoindium(I) compound reported, is polymer consisting of zigzag chains of alternating indium atoms and cyclopentadienyl complexes.
Other oxidation states
Less frequently, indium forms compounds in oxidation state +2 and even fractional oxidation states. Usually such materials feature In–In bonding, most notably in halides, In2X4 and [In2X6]2−. Several other compounds are known to combine indium(I) and indium(III), such as InI6(InIIICl6)Cl3, InI5(InIIIBr4)2(InIIIBr6), InIInIIIBr4. In organic synthesis it is used for indium-mediated allylation.
Organoindium compounds feature In-C bonds. Most are In(III) derivatives, but cyclopentadienylindium(I) is an exception. Perhaps best known is trimethylindium, In(CH3)3, which is used to prepare certain semiconducting materials.
Biological and medical functions
Indium has no metabolic role in any organism. In a similar way to aluminium salts, indium(III) ions can be toxic to the kidney when given by injection, but oral indium compounds do not have the chronic toxicity of salts of heavy metals, probably due to poor absorption in basic conditions. Radioactive indium-111 (in very small amounts on a chemical basis) is used in nuclear medicine tests, as a radiotracer to follow the movement of labeled proteins and white blood cells in the body.
Indium is created via the long-lasting, (up to thousands of years), s-process in low-to-medium mass stars (which range in mass between 0.6 and 10 solar masses). When a silver-109 atom (the isotope of which approximately half of all silver in existence is composed), catches a neutron, it undergoes a beta decay to become cadmium-110. Capturing further neutrons, it becomes cadmium-115, which decays to indium-115 via another beta decay. This explains why the radioactive isotope predominates in abundance compared to the stable one.
In Earth's crust, indium occurs only in the form of its compounds, except occasionally as rare grains of free metal of no commercial importance. Indium is 68th most abundant element in Earth's crust at approximately 160 ppb, making indium approximately as abundant as cadmium. Fewer than 10 indium minerals are known, such as dzhalindite (In(OH)3) and indite (FeIn2S4), but none of these occurs in significant deposits.
Based on content of indium in zinc ore stocks, there is a worldwide reserve of approximately 6,000 tonnes of economically viable indium. However, the Indium Corporation, the largest processor of indium, claims that, on the basis of increasing recovery yields during extraction, recovery from a wider range of base metals (including tin, copper and other polymetallic deposits) and new mining investments, the long-term supply of indium is sustainable, reliable, and sufficient to meet increasing future demands. This conclusion may be reasonable considering that silver, which is one-third as abundant as indium in Earth's crust, is currently mined at approximately 18,300 tonnes per year, which is 40 times greater than current indium mining rates.
In 1863, the German chemists Ferdinand Reich and Hieronymous Theodor Richter were testing ores from the mines around Freiberg, Saxony. They dissolved the minerals pyrite, arsenopyrite, galena and sphalerite in hydrochloric acid and distilled raw zinc chloride. As it was known that ores from that region sometimes contain thallium they searched for the green emission lines with spectroscopy. The green lines were absent but a blue line was present in the spectrum. As no element was known with a bright blue emission they concluded that a new element was present in the minerals. They named the element with the blue spectral line indium, from the indigo color seen in its spectrum. That line was the first indication of an unknown element in zinc ores, and when the free metal was isolated in the following year it was named indium after the colour of the light that had provided a clue to its presence. Zinc ores remain the primary source of indium.
In 1924, indium was found to have a valued ability to stabilize non-ferrous metals, which was the first significant use for the element. It took until 1936 for the U.S. Bureau of Mines to list indium as a commodity, and even in the early 1950s only very limited applications for indium were known, the most important of which was making light-emitting diodes and coating bearings for aircraft engines during World War II. The start of production of indium-containing semiconductors started in 1952. The development and widespread use of indium-containing nuclear control rods increased demand during the 1970s, and the use of indium tin oxide in liquid crystal displays increased and became the major application by 1992.
Currently the demand for indium is driven by the manufacture of transparent electrodes from indium tin oxide (ITO). The electrodes are used in liquid crystal displays and touchscreens. The metal also is used in a wide range of alloys; one of its first large-volume applications was in high-performance bearing alloys (for aircraft) in WWII. It is also used for making particularly low melting point alloys, and is a component in some solders. One of its unusual attributes is that, like gallium molten indium wets glass, so that it can be used as a solder in glass seals. It also is used in a wide range of electric and electronic roles, and has been used in superconducting alloys.
The lack of indium mineral deposits and the fact that indium is enriched in sulfidic lead, tin, copper, iron and predominately in zinc deposits, makes zinc production the main source for indium. The indium is leached from slag and dust of zinc production. Further purification is done by electrolysis. The exact process varies with the exact composition of the slag and dust.
Indium is produced mainly from residues generated during zinc ore processing but is also found in iron, lead, and copper ores. China is a leading producer of indium (390 tonnes in 2012), followed by Canada, Japan and South Korea with 70 tonnes each. The Teck Cominco refinery in Trail, British Columbia, is a large single-source indium producer, with an output of 32.5 tonnes in 2005, 41.8 tonnes in 2004 and 36.1 tonnes in 2003. South American Silver Corporation's Malku Khota property in Bolivia is a large resource of indium with an indicated resource of 1,481 tonnes and inferred resource of 935 tonnes. Adex Mining Inc.’s Mount Pleasant Mine in New Brunswick, Canada, holds some of the world’s total known indium resources.
The amount of indium consumed is largely a function of worldwide LCD production. Worldwide production in 2007 was 475 tonnes per year from mining and a further 650 tonnes per year from recycling. Demand has risen rapidly in recent years with the popularity of LCD computer monitors and television sets, which now account for 50% of indium consumption. Increased manufacturing efficiency and recycling (especially in Japan) maintain a balance between demand and supply. According to the UNEP, indium's end-of-life recycling rate is less than 1%. Demand increased as the metal is used in LCDs and televisions, and supply decreased when a number of Chinese mining concerns stopped extracting indium from their zinc tailings. In 2002, the price was US$94 per kilogram. The recent changes in demand and supply have resulted in high and fluctuating prices of indium, which from 2006 to 2009 ranged from US$382/kg to US$918/kg.
The first large-scale application for indium was as a coating for bearings in high-performance aircraft engines during World War II. Afterward, production gradually increased as new uses were found in fusible alloys, solders, and electronics. In the 1950s, tiny beads of it were used for the emitters and collectors of PNP alloy junction transistors. In the middle and late 1980s, the development of indium phosphide semiconductors and indium tin oxide thin films for liquid crystal displays (LCD) aroused much interest. By 1992, the thin-film application had become the largest end use.
- Indium oxide (In2O3) and indium tin oxide (ITO) are used as a transparent conductive coating applied to glass substrates in the making of electroluminescent panels.
- Some indium compounds such as indium antimonide, indium phosphide, and indium nitride are semiconductors with useful properties.
- Indium is used in photovoltaics for the synthesis of the semiconductor copper indium gallium selenide (CIGS), which is used for the manufacture of CIGS solar cells, a type of second generation thin film solar cell.
- Used in light-emitting diodes (LEDs) and laser diodes based on compound semiconductors such as InGaN, InGaP that are fabricated by Metalorganic Vapor Phase Epitaxy (MOVPE) technology.
- Ultrapure metalorganics of indium include high purity trimethylindium (TMI), which is used as a precursor in III–V compound semiconductors, whereas it is also used as the semiconductor dopant in II–VI compound semiconductors.
- One of many substitutes for mercury in alkaline batteries to prevent the zinc from corroding and releasing hydrogen gas.
Metal and alloys
- Very small amounts used in aluminium alloy sacrificial anodes (for salt water applications) to prevent passivation of the aluminium.
- To bond gold electrical test leads to superconductors, indium is used as a conducting adhesive and applied under a microscope with precision tweezers.
- In the form of a wire it is used as a vacuum seal and a thermal conductor in cryogenics and ultra-high-vacuum applications, for example, in manufacturing gaskets that deform to fill gaps.
- Used as a calibration material for differential scanning calorimetry.
- It is an ingredient in the gallium–indium–tin alloy galinstan, which is liquid at room temperature but not toxic like mercury.
- Indium soldering is the preferred method to create a stress-free electrically and thermally conducting bond between a ceramic sputter target and a target holder.
- Indium tin oxide is used as a light filter in low-pressure sodium vapor lamps. The infrared radiation is reflected back into the lamp, which increases the temperature within the tube and therefore improves the performance of the lamp.
- Indium is a component of some dental amalgam alloys, in order to decrease the surface tension of the mercury and allow for less mercury and easier amalgamation.
- Indium's melting point of 429.7485 K (156.5985 °C) is a defining fixed point on the international temperature scale ITS-90.
- Indium's high neutron capture cross section for thermal neutrons makes it suitable for use in control rods for nuclear reactors, typically in an alloy containing 80% silver, 15% indium, and 5% cadmium.
- In nuclear engineering, the (n,n') reactions of 113In and 115In are used to determine magnitudes of neutron fluxes.
- Indium is also used as a thermal interface material by personal computer enthusiasts in the form of pre-shaped foil sheets fitted between the heat-transfer surface of a microprocessor and its heat sink. The application of heat partially melts the foil and allows the indium metal to fill in any microscopic gaps and pits between the two surfaces, removing any insulating air pockets that would otherwise compromise heat transfer efficiency.
- 111In emits gamma radiation and is used in indium leukocyte imaging, or indium scintigraphy, a technique of medical imaging that is particularly helpful in differentiating conditions such as osteomyelitis from decubitus ulcers for assessment of route and duration of antibiotic therapy. Indium leukocyte scintigraphy has many applications, including early phase drug development, and the monitoring of activity of white blood cells. For the test, blood is taken from the patient, white cells removed, labeled with the radioactive 111In, then re-injected back into the patient. Gamma imaging will then reveal any areas of on-going white-cell localization such as new and developing areas of infection.
The health effects of exposure to Indium have been little studied. The EU does not consider it a chemical of "high concern". Indium tin oxide and indium phosphide have been shown to cause harm to the pulmonary and immune systems, predominantly through ionic indium. Mild eye irritation may result from exposure to its dust or vapor. Lab studies in animals have shown injection may cause liver and kidney damage. Because of its rarity, little is known about its ecological fate, and bioaccumulation has not been ruled out.
People can be exposed to indium in the workplace by breathing it in, swallowing it, skin contact, and eye contact. The National Institute for Occupational Safety and Health has set a recommended exposure limit (REL) of 0.1 mg/m3 over an 8-hour workday.
- Standard Atomic Weights 2013. Commission on Isotopic Abundances and Atomic Weights
- Mangum, B W (1989). "Determination of the Indium Freezing-point and Triple-point Temperatures". Metrologia. 26 (4): 211. Bibcode:1989Metro..26..211M. doi:10.1088/0026-1394/26/4/001.
- Guloy, A. M.; Corbett, J. D. (1996). "Synthesis, Structure, and Bonding of Two Lanthanum Indium Germanides with Novel Structures and Properties". Inorganic Chemistry. 35 (9): 2616–22. doi:10.1021/ic951378e.
- Lide, D. R., ed. (2005). "Magnetic susceptibility of the elements and inorganic compounds". CRC Handbook of Chemistry and Physics (PDF) (86th ed.). Boca Raton (FL): CRC Press. ISBN 0-8493-0486-5.
- W. M. Haynes (2010). David R. Lide, ed. CRC Handbook of Chemistry and Physics: A Ready-reference Book of Chemical and Physical Data. CRC Press. ISBN 978-1-4398-2077-3.
- Alfantazi, A. M.; Moskalyk, R. R. (2003). "Processing of indium: a review". Minerals Engineering. 16 (8): 687–694. doi:10.1016/S0892-6875(03)00168-7.
- Binder, Harry H. (1999). Lexicon der chemischen Elemente (in Deutsch). S. Hirzel Verlag. ISBN 3-7776-0736-3.
- Dean, John A. (523). Lange's handbook of chemistry (Fifteenth edition). McGraw-Hill, Inc. ISBN 0-07-016190-9.
- Greenwood, Norman N.; Earnshaw, Alan (1997). Chemistry of the Elements (2nd ed.). Butterworth-Heinemann. ISBN 0-08-037941-9.
- Audi, Georges; Bersillon, O.; Blachot, J.; Wapstra, A.H. (2003). "The NUBASE Evaluation of Nuclear and Decay Properties". Nuclear Physics A. Atomic Mass Data Center. 729: 3–128. Bibcode:2003NuPhA.729....3A. doi:10.1016/j.nuclphysa.2003.11.001.
- Holleman, Arnold F.; Wiberg, Egon; Wiberg, Nils (1985). "Thallium". Lehrbuch der Anorganischen Chemie (in Deutsch) (91–100 ed.). Walter de Gruyter. pp. 892–893. ISBN 3-11-007511-3.
- Haynes, William M., ed. (2011). CRC Handbook of Chemistry and Physics (92nd ed.). Boca Raton, FL: CRC Press. p. 8.20. ISBN 1439855110.
- Fischer, E. O.; Hofmann, H. P. (1957). "Metall-cyclopentadienyle des Indiums". Angewandte Chemie (in German). 69 (20): 639–640. doi:10.1002/ange.19570692008.
- Sinclair, Ian; Worrall, Ian J. (1982). "Neutral complexes of the indium dihalides". Canadian Journal of Chemistry. 60 (6): 695–698. doi:10.1139/v82-102.
- Beck, Horst Philipp; Wilhelm, Doris (1991). "In7Cl9—A New"Old" Compound in the System In-Cl". Angewandte Chemie International Edition in English. 30 (7): 824–825. doi:10.1002/anie.199108241.
- Dronskowski, Richard (1995). "Synthesis, Structure, and Decay of In4Br7". Angewandte Chemie International Edition in English. 34 (10): 1126–1128. doi:10.1002/anie.199511261.
- Boothroyd, A. I. (2006). "Heavy elements in stars". Science. 314 (5806): 1690–1691. PMID 17170281. doi:10.1126/science.1136842.
- "Abundance in Earth's Crust". WebElements.com. Archived from the original on 9 March 2007. Retrieved 2007-04-14.
- Sutherland, J. K. (1971). "A second occurrence of dzhalindite". The Canadian Mineralogist. 10 (5): 781–786.
- "Mineral Commodities Summary 2007: Indium" (PDF). United States Geological Survey. Retrieved 2007-12-26.
- "Indium and Gallium Supply Sustainability September 2007 Update". 22nd EU PV Conference, Milan, Italy. Archived from the original (PDF) on 28 December 2008. Retrieved 2007-12-26.
- "Indium Price Supported by LCD Demand and New Uses for the Metal". September 6, 2009.
- "Top World Silver Producers" (PDF). World Silver Survey 2007.
- Reich, F.; Richter, T. (1863). "Ueber das Indium". Journal für Praktische Chemie (in German). 90 (1): 172–176. doi:10.1002/prac.18630900122.
- Venetskii, S. (1971). "Indium". Metallurgist. 15 (2): 148–150. doi:10.1007/BF01088126.
- Reich, F.; Richter, T. (1864). "Ueber das Indium". Journal für Praktische Chemie (in German). 92 (1): 480–485. doi:10.1002/prac.18640920180.
- Schwarz-Schampera, Ulrich; Herzig, Peter M. (2002). Indium: Geology, Mineralogy, and Economics. Springer. ISBN 978-3-540-43135-0.
- French, Sidney J. (1934). "A story of indium". Journal of Chemical Education. 11 (5): 270. Bibcode:1934JChEd..11..270F. doi:10.1021/ed011p270.
- Schwarz-Schampera, Ulrich; Herzig, Peter M; Rohstoffe, Bundesanstalt für Geowissenschaften und (2002-06-10). "history". Indium: Geology, mineralogy, and economics. p. 1. ISBN 978-3-540-43135-0.
- Weeks, R.A. (1973). "Gallium, germanium, and indium". In Brobst, Donald Albert; Pratt, Walden P. Mines and mineral resources (PDF). pp. 237–246.
- Jorgenson, John D.; George, Micheal W. "Mineral Commodity Profile Indium" (PDF). United States Geological Survey.
- "Canadian Minerals Yearbook" (PDF). 2007. Archived from the original (PDF) on 2011-09-27.
- "Recycling Rates of Metals: A Status Report" (PDF). United Nations Environmental Programme. Retrieved August 2, 2011.
- Fathi Habashi (21 November 2008). Alloys: Preparation, Properties, Applications. John Wiley & Sons. pp. 294–. ISBN 978-3-527-61192-8.
- U.S. Geological Survey – Historical Statistics for Mineral and Material Commodities in the United States; INDIUM STATISTICS // USGS, April 1, 2014
- Tolcin, Amy C. (2013) Indium. USGS Mineral Commodity Summaries.
- "Malku Khota Updated Preliminary Economic Assessment, May 2011" (PDF). South American Silver Corp. Archived from the original (PDF) on 2012-01-19.
- Wright, Philip (1996). "Mineral and Metal Commodity Review: Tin" (PDF). Natural Resources Canada.
- "Indium Price Supported by LCD Demand and New Uses for the Metal" (PDF). Geology.com. Retrieved 2007-12-26.
- "USGS Mineral Commodity Summaries 2011" (PDF). USGS and USDI. Retrieved August 2, 2011.
- "How much is left?". ScientificAmerican. Retrieved 16 January 2013.
- Tolcin, Amy C. "Mineral Yearbook 2007: Indium" (PDF). United States Geological Survey.
- Downs, Anthony John (1993). Chemistry of Aluminium, Gallium, Indium, and Thallium. Springer. pp. 89 and 106. ISBN 978-0-7514-0103-5.
- "The Electroluminescent Light Sabre". Nanotechnology News Archive. Azonano. June 2, 2005. Retrieved 2007-08-29.
- Bachmann, K. J. (1981). "Properties, Preparation, and Device Applications of Indium Phosphide". Annual Review of Materials Science. 11: 441–484. Bibcode:1981AnRMS..11..441B. doi:10.1146/annurev.ms.11.080181.002301.
- Bhuiyan, Ghani; Hashimoto, Akihiro; Yamamoto, Akioare (2003). "Indium nitride (InN): A review on growth, characterization, and properties". Journal of Applied Physics. 94 (5): 2779. Bibcode:2003JAP....94.2779B. doi:10.1063/1.1595135.
- Powalla, M.; Dimmler, B. (2000). "Scaling up issues of CIGS solar cells". Thin Solid Films. 361–362: 540–546. Bibcode:2000TSF...361..540P. doi:10.1016/S0040-6090(99)00849-4.
- Schubert, E. Fred (2003). Light-Emitting Diodes. Cambridge University Press. p. 16. ISBN 0-521-53351-1.
- Shenai, Deodatta V.; Timmons, Michael L.; DiCarlo Jr., Ronald L.; Marsman, Charles J. (2004). "Correlation of film properties and reduced impurity concentrations in sources for III/V-MOVPE using high-purity trimethylindium and tertiarybutylphosphine". Journal of Crystal Growth. 272 (1–4): 603–608. Bibcode:2004JCrGr.272..603S. doi:10.1016/j.jcrysgro.2004.09.006.
- Geological Survey (U.S.) (2010). Minerals Yearbook, 2008, V. 1, Metals and Minerals. Government Printing Office. pp. 35–2. ISBN 978-1-4113-3015-3.
- Rabilloud, Guy (1997). High-performance Polymers: Conductive adhesives. Editions TECHNIP. p. 263. ISBN 2-7108-0716-5.
- Weissler, G. L., ed. (1990). "Vacuum physics and technology". San Diego: Acad. Press: 296. ISBN 978-0-12-475914-5.
- Reading, Mike; Hourston, Douglas J. (2006). Modulated temperature differential scanning calorimetry. Springer. p. 245. ISBN 978-1-4020-3749-8.
- Surmann, P; Zeyat, H (Nov 2005). "Voltammetric analysis using a self-renewable non-mercury electrode". Analytical and Bioanalytical Chemistry. 383 (6): 1009–13. PMID 16228199. doi:10.1007/s00216-005-0069-7.
- Weber, Dieter. "Bonding ceramic sputter targets to metal holders". Retrieved 19 October 2014.
- Powell LV, Johnson GH, Bales DJ (1989). "Effect of Admixed Indium on Mercury Vapor Release from Dental Amalgam". Journal of Dental Research. 68 (8): 1231–3. PMID 2632609. doi:10.1177/00220345890680080301.
- Preston-Thomas, H. (1990). "Procès-Verbaux du Comité International des Poids et Mesures". Metrologia. 27 (1): 3–10. Bibcode:1990Metro..27....3P. doi:10.1088/0026-1394/27/1/002.
- Scoullos, Michael J (2001-12-31). "Other types of cadmium alloys". Mercury, cadmium, lead: handbook for sustainable heavy metals policy and regulation. p. 222. ISBN 978-1-4020-0224-3.
- Berger, Harold; National Bureau Of Standards, United States; Committee E-7 On Nondestructive Testing, American Society for Testing and Materials (1976). "Image Detectors for Other Neutron Energies". Practical applications of neutron radiography and gaging: a symposium. pp. 50–51.
- Tong, Xingcun Colin (2011). Advanced Materials for Thermal Management of Electronic Packaging. Springer. p. 323. ISBN 978-1-4419-7759-5.
- Van Nostrand, D.; Abreu, S. H.; Callaghan, J. J.; Atkins, F. B.; Stoops, H. C.; Savory, C. G. (May 1988). "In-111-labeled white blood cell uptake in noninfected closed fracture in humans: prospective study". Radiology. 167 (2): 495–498. PMID 3357961. doi:10.1148/radiology.167.2.3357961.
- Gwinn, W. M.; Qu, W; Bousquet, R. W.; Price, H; Shines, C. J.; Taylor, G. J.; Waalkes, M. P.; Morgan, D. L. (2014). "Macrophage Solubilization and Cytotoxicity of Indium-Containing Particles as in vitro Correlates to Pulmonary Toxicity in vivo". Toxicological Sciences. 144 (1): 17–26. PMC . PMID 25527823. doi:10.1093/toxsci/kfu273.
- "CDC - NIOSH Pocket Guide to Chemical Hazards - Indium". www.cdc.gov. Retrieved 2015-11-06. line feed character in
|title=at position 47 (help)
- Indium at The Periodic Table of Videos (University of Nottingham)
- Reducing Agents > Indium low valent
- NIOSH Pocket Guide to Chemical Hazards (Centers for Disease Control and Prevention)
|Periodic table (Large cells)|